A Study on the Weldment Hardening Discrimination Procedure and Improvement of Flux Cored Arc Welding Process of ASTM A553-1 (9% Nickel Steel) Material Using Bead Geometry Distribution

: As a result of strengthened sulfur content standards for ship fuel oil in IMO regulations, major domestic and foreign carriers have a high and growing demand for liqueﬁed natural gas (LNG) powered ships and related equipment. For LNG operation in a cryogenic environment, a storage tank and fuel supply system that uses steel with excellent brittleness and fatigue strength is required. Ships that use LNG have a high vulnerability to explosion and ﬁre. For this reason, 9% Ni is typically used, since a ship requires high quality products with special materials and structural technologies that guarantee operability at cryogenic temperatures. However, there is an urgent need for research to derive a uniform welding quality, since high process difﬁculty and differences in welding quality related to a welder’s skills can cause a deterioration of the weld quality in the 9% Ni steel welding process. For 9% Ni steel, the higher the dilution ratio of the base metal, the lower the strength. In order to secure the required strength, excessive dilution of the base metal should be avoided, and the relationship between dilution ratio and strength should be investigated. According to previous research, if it exceeds 25% it may be lower than the API standard of 363 MPa for hardening welds. Therefore, in this study, the ﬂux cored arc welding process is performed by establishing criteria that can be evaluated based on the SVM method in order to determine the structure of the weld to be cured according to the dilution rate of the base metal. We would like to propose a multipurpose optimization algorithm to ensure uniform quality of 9% Ni steel.


Introduction
Since January 2020, the International Maritime Organization (IMO) has been applying a stricter standard for the sulfur content of ship fuel oil, finally announcing a plan to restrict the sulfur content of ship fuel oil from the current level of 3.5% to 0.5% in 2020. Around the world, each country has legislated the IMO 2020 standards, and is applying more stringent regulations to voluntarily designated emission control areas rather than other sea areas. Major domestic and international carriers are complying with IMO's strict environmental regulations by considering the pros and cons of various alternatives such as installing a scrubber, using low-sulfur oil, or using LNG.
As eco-friendliness has become an international trend, a dramatic energy transition is taking place around the world and the demand for liquefied natural gas (LNG) is also In previous studies, the correlation between diverse variables and mechanical characteristics applied to the welding process of cryogenic steels such as STS series or Ni alloy series has been reviewed and the process problems and quality deterioration that occurred when those were used in the LNG-related equipment were also reviewed. However, the previous research on weldment quality in cryogenic steel has not reflected the complex alternating effects, and most studies concern the application of automation, high melting, or high speeds to compensate for the disadvantages of manual welding [17,18]. In addition, research on the correlation between bead geometry and weldability has been performed in previous studies to improve welding quality by establishing the key factors affecting bead formation. However, similar size areas and heat-affected zones are derived intermittently even for different welding process variables, so the applicability of analysis and consideration limited to bead geometry in the actual field has been reduced.
In this way, an analysis based on various perspectives is needed to clearly identify the specific conditions that can have a similar bead geometry compared to the intermittent variables, and it is necessary to identify the phenomenon in which the structure of a weldment is hardened by matching the characteristics generated from the correlation between the partially divided bead geometry within a weldment to the dilution ratio of a weldment.
In 9% Ni steel, a higher dilution ratio of the base material leads to lower strength. For this reason, to guarantee the required strength, excessive dilution of the base material should be avoided. Although prior studies on the correlation between dilution ratio and strength have found that tensile strength does not change dramatically even when there is 10-20% change in the dilution ratio, it has been reported that strength may drop below the API standard of 363 MPa due to the hardening of the weldment if the dilution ratio is 25% or more [19,20].
Therefore, in this study, the dilution ratio formed in the weldment was calculated for the flux cored arc welding process applied to 9% Ni, a cryogenic steel, and the phenomenon in which a hardened weldment is created compared to the heat-affected zone was identified in a procedure based on the calculated dilution ratio. This study tried with purpose a method for quantitatively evaluating the quality of weldments. Therefore, the bead geometry, hardness, and dilution rate were analyzed for the welded part (which was tested by applying various process variables), and the correlation of the tendency of the quality of the welded part to deteriorate was derived. In addition, the raw data collected to quantify the quality deterioration characteristics of the collected welds was trained by the discriminant function. The effects contained in the process variables were predicted, and the quality deterioration characteristics were based on the process variables [21][22][23]. If this as expected, we have also proposed a multipurpose algorithm that can be systematically avoided.

Experimental Works
A flux cored arc welding experiment was carried out to determine the quality of flux cored arc weld of 9% Ni steel and to develop the optimal process parameters. For the experiment, a 600A class FCAW welding machine (ProPAC, HYOSUNG, Mapo-gu, Seoul, Korea) and torch, a welding feeder, a straight welding carriage, and a guide rail were configured, and the overall system was arranged as shown in Figure 1.
The specimen was cleaned with ethyl alcohol (DUKSAN, Ansan-si, Gyeonggi-do, Korea) and sandpaper to prevent foreign substances such as rust, scale, and oxide from causing welding defects on the surface of a specimen to be welded. Figure 2 shows the schematic diagram of a flux cored arc welding process. The test piece used in the welding test was used in a size of 150 mm (W) × 200 mm (H) × 15 mm (H) of 9% Ni steel (NIPPON STEEL, Chiyoda City, Tokyo, Japan). The mechanical properties and chemical composition of the 9% Ni steel and wire used in the flux cored arc welding test are shown in Tables 1 and 2, respectively. The specimen was cleaned with ethyl alcohol (DUKSAN, Ansan-si, Gyeonggi-do, Korea) and sandpaper to prevent foreign substances such as rust, scale, and oxide from causing welding defects on the surface of a specimen to be welded. Figure 2 shows the schematic diagram of a flux cored arc welding process. The test piece used in the welding test was used in a size of 150 mm (W) × 200 mm (H) × 15 mm (H) of 9% Ni steel (NIPPON STEEL, Chiyoda City, Tokyo, Japan). The mechanical properties and chemical composition of the 9% Ni steel and wire used in the flux cored arc welding test are shown in Tables 1 and 2, respectively.    The specimen was cleaned with ethyl alcohol (DUKSAN, Ansan-si, Gyeonggi-do, Korea) and sandpaper to prevent foreign substances such as rust, scale, and oxide from causing welding defects on the surface of a specimen to be welded. Figure 2 shows the schematic diagram of a flux cored arc welding process. The test piece used in the welding test was used in a size of 150 mm (W) × 200 mm (H) × 15 mm (H) of 9% Ni steel (NIPPON STEEL, Chiyoda City, Tokyo, Japan). The mechanical properties and chemical composition of the 9% Ni steel and wire used in the flux cored arc welding test are shown in Tables 1 and 2, respectively.    The selected input variables of flux cored arc welding applied in this experiment were welding current, arc voltage, and welding speed, which have a clear influence on the bead geometry and weldability of GMA weldment. To analyze the weldability, bead geometry and mechanical properties such as heat-affected zone and weldment hardness were collected [11]. Figure 3 shows the schematic diagram for the measurement of a penetration bead of the weldment. The selected input variables of flux cored arc welding applied in this experiment were welding current, arc voltage, and welding speed, which have a clear influence on the bead geometry and weldability of GMA weldment. To analyze the weldability, bead geometry and mechanical properties such as heat-affected zone and weldment hardness were collected [11]. Figure 3 shows the schematic diagram for the measurement of a penetration bead of the weldment. In this experiment, it is possible to estimate all factor effects for the response of an output variable according to the change of an input variable, and the full factorial placement method (FFD) was applied to detect the correlation effect of higher orders. The appropriate level and range of input variables (welding current, arc voltage, welding speed) were selected from preliminary experiments. A total of 18 experimental conditions were created from 3 2 × 2 (three welding current, three arc voltage, and two welding speed). Tables 3 and 4 show the experimental variables and levels of the input variables and the experimental conditions for a total of 18 trials.  In this experiment, it is possible to estimate all factor effects for the response of an output variable according to the change of an input variable, and the full factorial placement method (FFD) was applied to detect the correlation effect of higher orders. The appropriate level and range of input variables (welding current, arc voltage, welding speed) were selected from preliminary experiments. A total of 18 experimental conditions were created from 3 2 × 2 (three welding current, three arc voltage, and two welding speed). Tables 3 and 4 show the experimental variables and levels of the input variables and the experimental conditions for a total of 18 trials.

Measurement of Bead Geometry
BOP flux cored arc welding of 9% Ni steel, which is a cryogenic steel, was performed properly according to the process parameters. In the result of the experiment, it was confirmed that a good weldment was formed in general and there were no pores or defects in appearance. To properly represent the cross-sectional appearance of a specimen, 90% Ethanol + 10% Nitric solution was mixed and used to etch the cross-section. An optical microscope system was used to measure the bead geometry accurately. Table 5 shows the welding cross-section and bead measurement results taken with a 10X optical microscope (Sometech, Seoul, Korea).

Measurement of Bead Geometry
BOP flux cored arc welding of 9% Ni steel, which is a cryogenic steel, was performed properly according to the process parameters. In the result of the experiment, it was confirmed that a good weldment was formed in general and there were no pores or defects in appearance. To properly represent the cross-sectional appearance of a specimen, 90% Ethanol + 10% Nitric solution was mixed and used to etch the cross-section. An optical microscope system was used to measure the bead geometry accurately. Table 5 shows the welding cross-section and bead measurement results taken with a 10X optical microscope (Sometech, Seoul, Korea).

Measurement of Bead Geometry
BOP flux cored arc welding of 9% Ni steel, which is a cryogenic steel, was performed properly according to the process parameters. In the result of the experiment, it was confirmed that a good weldment was formed in general and there were no pores or defects in appearance. To properly represent the cross-sectional appearance of a specimen, 90% Ethanol + 10% Nitric solution was mixed and used to etch the cross-section. An optical microscope system was used to measure the bead geometry accurately. Table 5 shows the welding cross-section and bead measurement results taken with a 10X optical microscope (Sometech, Seoul, Korea).

Measurement of Bead Geometry
BOP flux cored arc welding of 9% Ni steel, which is a cryogenic steel, was performed properly according to the process parameters. In the result of the experiment, it was confirmed that a good weldment was formed in general and there were no pores or defects in appearance. To properly represent the cross-sectional appearance of a specimen, 90% Ethanol + 10% Nitric solution was mixed and used to etch the cross-section. An optical microscope system was used to measure the bead geometry accurately. Table 5 shows the welding cross-section and bead measurement results taken with a 10X optical microscope (Sometech, Seoul, Korea).

Measurement of Bead Geometry
BOP flux cored arc welding of 9% Ni steel, which is a cryogenic steel, was performed properly according to the process parameters. In the result of the experiment, it was confirmed that a good weldment was formed in general and there were no pores or defects in appearance. To properly represent the cross-sectional appearance of a specimen, 90% Ethanol + 10% Nitric solution was mixed and used to etch the cross-section. An optical microscope system was used to measure the bead geometry accurately. Table 5 shows the welding cross-section and bead measurement results taken with a 10X optical microscope (Sometech, Seoul, Korea).

Measurement of Weldment Hardness
A hardness test was performed on each specimen to confirm the hardening phenomenon of a weldment where there is a change of internal strength and structure due to the difference in the concentration of the arc force and the electromagnetic force when the flux cored arc weldment was solidified. To determine the hardness of a weldment, the Vickers hardness test was performed on the upper and lower parts and the heat-affected zone where the change in internal strength occurs. The load used in the hardness test was selected as 0.5 N and analysis was performed at 0.83 mm intervals so as not to affect the nearby hardness. Figure 4 shows the schematic diagram of the hardness test for the weldment of 9% Ni steel. Table 6 shows the test results for the hardness of upper and lower parts of a weldment and the heat-affected zone. The hardness test result means the average value measured at 5 points. The hardness (lower part) of a flux cored arc weldment shows a value between 286.1 HV0.05 and 291.9 HV0.05, which is higher than the 243 HV0.05 hardness which is a 9% Ni steel standard. Therefore, it is judged that sufficient weldability is achieved. 17 12

Measurement of Weldment Hardness
A hardness test was performed on each specimen to confirm the hardening phenomenon of a weldment where there is a change of internal strength and structure due to the difference in the concentration of the arc force and the electromagnetic force when the flux cored arc weldment was solidified. To determine the hardness of a weldment, the Vickers hardness test was performed on the upper and lower parts and the heat-affected zone where the change in internal strength occurs. The load used in the hardness test was selected as 0.5 N and analysis was performed at 0.83 mm intervals so as not to affect the nearby hardness. Figure 4 shows the schematic diagram of the hardness test for the weldment of 9% Ni steel. Table 6 shows the test results for the hardness of upper and lower parts of a weldment and the heat-affected zone. The hardness test result means the average value measured at 5 points. The hardness (lower part) of a flux cored arc weldment shows a value between 286.1 HV0.05 and 291.9 HV0.05, which is higher than the 243 HV0.05 hardness which is a 9% Ni steel standard. Therefore, it is judged that sufficient weldability is achieved. 18 13

Measurement of Weldment Hardness
A hardness test was performed on each specimen to confirm the hardening phenomenon of a weldment where there is a change of internal strength and structure due to the difference in the concentration of the arc force and the electromagnetic force when the flux cored arc weldment was solidified. To determine the hardness of a weldment, the Vickers hardness test was performed on the upper and lower parts and the heat-affected zone where the change in internal strength occurs. The load used in the hardness test was selected as 0.5 N and analysis was performed at 0.83 mm intervals so as not to affect the nearby hardness. Figure 4 shows the schematic diagram of the hardness test for the weldment of 9% Ni steel. Table 6 shows the test results for the hardness of upper and lower parts of a weldment and the heat-affected zone. The hardness test result means the average value measured at 5 points. The hardness (lower part) of a flux cored arc weldment shows a value between 286.1 HV0.05 and 291.9 HV0.05, which is higher than the 243 HV0.05 hardness which is a 9% Ni steel standard. Therefore, it is judged that sufficient weldability is achieved.

Measurement of Weldment Hardness
A hardness test was performed on each specimen to confirm the hardening phenomenon of a weldment where there is a change of internal strength and structure due to the difference in the concentration of the arc force and the electromagnetic force when the flux cored arc weldment was solidified. To determine the hardness of a weldment, the Vickers hardness test was performed on the upper and lower parts and the heat-affected zone where the change in internal strength occurs. The load used in the hardness test was selected as 0.5 N and analysis was performed at 0.83 mm intervals so as not to affect the nearby hardness. Figure 4 shows the schematic diagram of the hardness test for the weldment of 9% Ni steel. Table 6 shows the test results for the hardness of upper and lower parts of a weldment and the heat-affected zone. The hardness test result means the average value measured at 5 points. The hardness (lower part) of a flux cored arc weldment shows a value between 286.1 HV0.05 and 291.9 HV0.05, which is higher than the 243 HV0.05 hardness which is a 9% Ni steel standard. Therefore, it is judged that sufficient weldability is achieved. Metals 2021, 11, x 8 of 18

Measurement of Weldment Dilution Ratio
The bead geometry of a flux cored arc welding process varies depending on the changes in arc force and heat input caused by differences in welding current, arc voltage, and wire supply speed. There is a very high possibility that hardening will occur due to a change in the chemical composition and internal strength of the weldment. In this way, the characteristics from the correlation between the bead geometry and the quality characteristics of a weldment were matched to the dilution ratio of a weldment in order to analyze the phenomenon of hardening of a weldment structure. Figure 5 shows the schematic diagram to calculate the weldment dilution ratio of a flux cored arc welding process and Figure 6 shows the picture of calculating a weldment dilution ratio using the area analysis tool in the system via an optical microscope. Table 7 shows the dilution ratio of the weldment area according to the flux cored arc welding process parameters.

Measurement of Weldment Dilution Ratio
The bead geometry of a flux cored arc welding process varies depending on the changes in arc force and heat input caused by differences in welding current, arc voltage, and wire supply speed. There is a very high possibility that hardening will occur due to a change in the chemical composition and internal strength of the weldment. In this way, the characteristics from the correlation between the bead geometry and the quality characteristics of a weldment were matched to the dilution ratio of a weldment in order to analyze the phenomenon of hardening of a weldment structure. Figure 5 shows the schematic diagram to calculate the weldment dilution ratio of a flux cored arc welding process and Figure 6 shows the picture of calculating a weldment dilution ratio using the area analysis tool in the system via an optical microscope. Table 7 shows the dilution ratio of the weldment area according to the flux cored arc welding process parameters.

Weldment Hardening According to Dilution Ratio
In 9% Ni steel, a higher dilution ratio of the base material results in lower strength. To secure the required strength, excessive dilution of the base material should thus be avoided. Although prior studies on the relationship between dilution ratio and strength

Weldment Hardening According to Dilution Ratio
In 9% Ni steel, a higher dilution ratio of the base material results in lower strength. To secure the required strength, excessive dilution of the base material should thus be avoided. Although prior studies on the relationship between dilution ratio and strength

Weldment Hardening According to Dilution Ratio
In 9% Ni steel, a higher dilution ratio of the base material results in lower strength. To secure the required strength, excessive dilution of the base material should thus be avoided. Although prior studies on the relationship between dilution ratio and strength have found that the tensile strength does not change significantly even when there is 10-20% change in dilution, it has been reported that it may be lower than the API standard of 363 MPa due to hardening of a weldment if dilution is 25% or more [19,20]. In addition, even under different welding conditions, the level of hardening of heat-affected zones is similar when the amount of heat input is the same. However, the electromagnetic force and the energy density of the beam are different, so the effect on bead formation is also different. This leads to a disadvantage of increased hardness of a weldment compared to the heat-affected zone. To address the shortcomings of prior studies that established the characteristics of a welding process limited to bead geometry as described above, the correlation between dilution concept and strength of a weldment was established.
Therefore, in this section, the dilution ratio formed in a weldment is calculated for each welding process and process variable and a standard for the generation of a weldment hardened compared to the heat-affected zone is established according to the calculated dilution ratio in order to set up a stable weldment dilution ratio standard.
To analyze the correlation of hardness based on the dilution ratio that changes according to the bead geometry, we attempted to establish a standard for hardening or scattering of the lower weldment compared to the heat-affected zone. The difference and trend between the measured hardness of the heat-affected zone and the hardness of the lower weldment were used to set up a dilution ratio standard that can avoid hardening of a weldment, as shown in Figure 7. As a result, the degree of hardness (i.e., the difference between the hardness of heat-affected zone and the hardness of lower weldment) of a flux cored arc weldment was between 42.8 HV0.05 and 58.7 HV0.05 and the difference in hardness of a weldment was confirmed to be 42.8 HV0.05 or lower compared to the heat-affected zone (when the dilution ratio of weldment was calculated to be 15.0% or more). It was thus confirmed that the difference in hardness compared to the heat affected zone was not high as the dilution ratio was increased. It was judged that if there is this kind of hardening of a weldment, it is difficult to secure the quality against the brittle effect and durability. have found that the tensile strength does not change significantly even when there is 10-20% change in dilution, it has been reported that it may be lower than the API standard of 363 MPa due to hardening of a weldment if dilution is 25% or more [19,20]. In addition, even under different welding conditions, the level of hardening of heat-affected zones is similar when the amount of heat input is the same. However, the electromagnetic force and the energy density of the beam are different, so the effect on bead formation is also different. This leads to a disadvantage of increased hardness of a weldment compared to the heat-affected zone. To address the shortcomings of prior studies that established the characteristics of a welding process limited to bead geometry as described above, the correlation between dilution concept and strength of a weldment was established. Therefore, in this section, the dilution ratio formed in a weldment is calculated for each welding process and process variable and a standard for the generation of a weldment hardened compared to the heat-affected zone is established according to the calculated dilution ratio in order to set up a stable weldment dilution ratio standard.
To analyze the correlation of hardness based on the dilution ratio that changes according to the bead geometry, we attempted to establish a standard for hardening or scattering of the lower weldment compared to the heat-affected zone. The difference and trend between the measured hardness of the heat-affected zone and the hardness of the lower weldment were used to set up a dilution ratio standard that can avoid hardening of a weldment, as shown in Figure 7. As a result, the degree of hardness (i.e., the difference between the hardness of heat-affected zone and the hardness of lower weldment) of a flux cored arc weldment was between 42.8 HV0.05 and 58.7 HV0.05 and the difference in hardness of a weldment was confirmed to be 42.8 HV0.05 or lower compared to the heat-affected zone (when the dilution ratio of weldment was calculated to be 15.0% or more). It was thus confirmed that the difference in hardness compared to the heat affected zone was not high as the dilution ratio was increased. It was judged that if there is this kind of hardening of a weldment, it is difficult to secure the quality against the brittle effect and durability. The standard of a 15.0% dilution ratio confirmed above is a standardized score, and can be used as an evaluation index for the process. When a high score is calculated, it means that a hardened structure of a weldment is created. Therefore, the criteria for determining the hardening of a weldment can be defined as shown in Table 8. These standardized scores can be later applied as learning data to determine the increase in weldment The standard of a 15.0% dilution ratio confirmed above is a standardized score, and can be used as an evaluation index for the process. When a high score is calculated, it means that a hardened structure of a weldment is created. Therefore, the criteria for determining the hardening of a weldment can be defined as shown in Table 8. These standardized scores can be later applied as learning data to determine the increase in weldment hardness and brittleness according to the bead geometry and dilution ratio. We attempted to prevent the generation of hardened structure and deterioration of weldment strength due to arc electromagnetic force at 9% Ni steel weldment where the welding process was applied.

Discriminant Analysis
The system to determine weldment hardening in the flux cored arc welding process of 9% Ni steel is a technique used to determine the affiliation of the input data by making a model using the collected data and entering it into the developed group learning data [24][25][26].
For the weldment hardening system to be developed in this study, a discriminant model was developed using the SVM (Support Vector Machine) technique. In the problem of finding the hyperplane that maximizes a margin in the two classes where linear discrimination is possible based on the VC (Vapnik-Chervonenkis) theory and Equation (1), this study tried to determine the possibility of hardening of a weldment in the process [27].
The variables for learning in the weldment hardening discrimination model are welding process variables (welding current, arc voltage, welding speed), bead geometry (topbead width, top-bead height), upper and bottom hardness, heat affected zone hardness (HAZ hardness), and dilution ratio. One hundred and eighty data points were entered with a total of 10 multiple variables. For the groups used to determine the hardening of a weldment, the Regard Group was defined as 1 and the Regardless Group was defined as 0, to confirm the discrimination performance predicted based on the SVM technique. Table 9 shows the learning data to discriminate the hardening of a weldment and Table 10 and Figure 8 quantitatively show the group discrimination performance which was predicted by the data learned in the SVM technique.

Development of Mathematical Model Welding Factors
The response surface analysis method is a statistical analysis method for the response surface formed by the change of response when several input variables , , , ⋯ have an effect on the output variable through complex actions. This procedure was carried out in the previous research [7].
The functional relationship between the input variables , , , ⋯ and the output variable is expressed by Equation (2). Considering the predictive ability of linear and nonlinear models, Equation (3) is expressed as a second order regression model if it is assumed the predicted value of the output variable (i.e., the welding factor) has a linear relationship with an input variable.

Development of Mathematical Model Welding Factors
The response surface analysis method is a statistical analysis method for the response surface formed by the change of response when several input variables x 1 , x 2 , x 3 , · · · x k have an effect on the output variable y through complex actions. This procedure was carried out in the previous research [7].
The functional relationship between the input variables x 1 , x 2 , x 3 , · · · x k and the output variable y is expressed by Equation (2). Considering the predictive ability of linear and nonlinear models, Equation (3) is expressed as a second order regression model if it is assumed the predicted value of the output variable (i.e., the welding factor) has a linear relationship with an input variable.
To obtain relevant data through experiments in this way, numerous trials and errors may occur, resulting in economic losses. To reduce these losses, a full factorial design was applied among the response surface analysis methods of the DOE method that well reflects the second order regression model, and the coefficients of each term were calculated using MINITAB.
The mathematical prediction models of bead geometry (top-bead width, top-bead height), upper and bottom hardness, HAZ hardness, and dilution ratio developed using regression coefficients and Equation (5) can be expressed using Equations (6)- (11).
To check the predictive ability of the developed mathematical prediction model, the graph showing the error range by comparing the average value of measured welding factors for each experimental condition with the predicted welding factors is shown in Figure 9. As shown in Table 11, the prediction model error range showed reliable results in general.
In addition, the ANOVA (analysis of variable) results of the predictive model confirmed a high coefficient of determination of 98.9% at the maximum bead width and a minimum coefficient of determination of 72.4% at the bottom hardness of a weldment. This means that it is possible to predict by using the coefficient of determination for the entire variation of welding factors, and the interaction as well as the independent influence of input variables affecting the regression model are considered simultaneously.

Optimization for Welding Process of 9% Ni Steel
The MOO (multi-objective optimization) algorithm to be applied in this study is a technique used to search for non-dominant solutions. This process is derived in previous research [7,[28][29][30]. The program schematic diagram of the MOO optimization method is shown in Figure 10, and MATLAB, which is a commercial numerical analysis program,

Optimization for Welding Process of 9% Ni Steel
The MOO (multi-objective optimization) algorithm to be applied in this study is a technique used to search for non-dominant solutions. This process is derived in previous research [7,[28][29][30]. The program schematic diagram of the MOO optimization method is shown in Figure 10, and MATLAB, which is a commercial numerical analysis program, was used to apply and modify the optimization method. To optimize the welding process variables where the hardening of a weldment has occurred, the same 180 data points in Table 9, which were learned in discriminant analysis, were used, and the variables and levels to drive the MOO optimization technique are shown in Table 12.
was used to apply and modify the optimization method. To optimize the welding process variables where the hardening of a weldment has occurred, the same 180 data points in Table 9, which were learned in discriminant analysis, were used, and the variables and levels to drive the MOO optimization technique are shown in Table 12.   [7], which used "solidification crack susceptibility" as the criteria of welding performance.
The objective function is a mathematical model of the characteristics of a system, and the constraint indicates the conditions that system variables can have. Therefore, Equations (12)- (14) represent the objective function ( ) of an arbitrary system having as a variable, and the constraints and ranges required to optimize this function [31].
Based on the optimization procedure built as described above, Tests No. 2 and 6 were selected to follow the MOO algorithm and Table 13 shows the welding process variables, expected welding factors, and discrimination results that have been modified to satisfy the constraints according to the optimization procedure.  Those conditions are as same as previous research [7], which used "solidification crack susceptibility" as the criteria of welding performance.
The objective function is a mathematical model of the characteristics of a system, and the constraint indicates the conditions that system variables can have. Therefore, Equations (12)- (14) represent the objective function f (x) of an arbitrary system having x as a variable, and the constraints and ranges required to optimize this function [31].
Based on the optimization procedure built as described above, Tests No. 2 and 6 were selected to follow the MOO algorithm and Table 13 shows the welding process variables, expected welding factors, and discrimination results that have been modified to satisfy the constraints according to the optimization procedure. Figure 11 tried to confirm the possibility of hardening of a weldment by applying the modified input variables, and the effectiveness of optimizing the welding process for 9% Ni steel was confirmed by performing a comparative analysis with the hardening of a weldment caused by the existing input variables. As a result, it was confirmed that the two raw data points selected in the flux cored arc welding process satisfy the dilution ratio of 15.0% or less, which is the limiting condition for hardening of a weldment, and the quality degradation characteristics appearing in the previous process variables were resolved by the modified process variables.   Figure 11 tried to confirm the possibility of hardening of a weldment by applying the modified input variables, and the effectiveness of optimizing the welding process for 9% Ni steel was confirmed by performing a comparative analysis with the hardening of a weldment caused by the existing input variables. As a result, it was confirmed that the two raw data points selected in the flux cored arc welding process satisfy the dilution ratio of 15.0% or less, which is the limiting condition for hardening of a weldment, and the quality degradation characteristics appearing in the previous process variables were resolved by the modified process variables. Figure 11. Weldment hardening distributions using modified input parameters.

Conclusions
This study attempted to optimize the welding process for 9% Ni steel, which is dominantly used in the LNG storage tank industry. After establishing the criteria for hardening of a weldment in the process, conducting learning in the discriminant function, and optimizing the process variables for hardening of a weldment using the discriminant group, the following conclusions were obtained: (1) Appropriate weldability of a weldment was confirmed by measuring the bead geometry, mechanical strength, welding area of a weldment derived from the flux cored arc welding test. It was found the hardening of a weldment depends on the concentration of arc electromagnetic force applied to the weldment and the ratio of an area mixed with a wire after melting. In addition, when a weldment hardening index of 15.0% or more is calculated, the group that needs to consider quality deterioration for weldment hardening is classified, so quality deterioration characteristics according to dilution ratio have been established. Figure 11. Weldment hardening distributions using modified input parameters.

Conclusions
This study attempted to optimize the welding process for 9% Ni steel, which is dominantly used in the LNG storage tank industry. After establishing the criteria for hardening of a weldment in the process, conducting learning in the discriminant function, and optimizing the process variables for hardening of a weldment using the discriminant group, the following conclusions were obtained: (1) Appropriate weldability of a weldment was confirmed by measuring the bead geometry, mechanical strength, welding area of a weldment derived from the flux cored arc welding test. It was found the hardening of a weldment depends on the concentration of arc electromagnetic force applied to the weldment and the ratio of an area mixed with a wire after melting. In addition, when a weldment hardening index of 15.0% or more is calculated, the group that needs to consider quality deterioration for weldment hardening is classified, so quality deterioration characteristics according to dilution ratio have been established. (2) To determine the weldment hardening phenomenon of 9% Ni steel caused by welding process variables, the quality deterioration characteristics were learned through the SVM technique, and it was determined whether the group with quality deterioration could be accurately identified. As a result, it was confirmed that a group with the hardening of a weldment was predicted 100% repeatedly. This result was reflected, and it was used as a procedure to determine the deterioration of weldment quality.
(3) A response surface method mathematical prediction model was developed to apply an objective function to optimize the welding process variables where quality deterioration occurs, and it was used in a multi-purpose optimization algorithm. The mathematical model for predicting each factor shows predictive performance in the range of 72.4% to 98.9%. The lowest performance of 72.4% was confirmed in the model predicting the hardness of the lower part of the weld, and the highest performance of 98.9% was confirmed in the model predicting the bead width. By entering the raw data of weldment hardening into the optimization algorithm created by the objective function and constraint conditions, the quality degradation characteristics contained in the process variables were supplemented. (4) Test No. 2 and 6 of Raw Data in which weld hardening occurred were selected and adjusted according to the MOO algorithm, and corrected to satisfy the dilution rate limiting condition by the optimization procedure. As a result of inputting the input variables complemented with the deterioration characteristics into the mathematical model of the reaction surface, calculating the predicted welding factor, and re-entering the output variables into the discrimination system, hardening of the welded part is expected. It was confirmed that the dilution rate of all the raw data was less than 15% and that the deterioration of quality was offset.